Altering polarization attributes in ferroelectric metallo-cavitands by varying hydrated alkali-metal guest cations
Srivastava, Anant Kumar; Vijayakanth, Thangavel; Divya, Pillutla; Praveenkumar, B.; Steiner, Alexander; Boomishankar, Ramamoorthy; Journal of Materials Chemistry C 5 (2017) 7352–; doi:10.1039/C7TC01758H

data_7236800
_publ_section_title
;
 Altering polarization attributes in ferroelectric metallo-cavitands by
 varying hydrated alkali-metal guest cations
;
_journal_issue                   29
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              7352
_journal_paper_doi               10.1039/C7TC01758H
_journal_volume                  5
_journal_year                    2017
_chemical_absolute_configuration unk
_chemical_formula_sum            'C128 H204 N40 Ni4 O74 P8'
_chemical_formula_weight         3969.90
_space_group_crystal_system      tetragonal
_space_group_IT_number           97
_space_group_name_Hall           'I 4 2'
_space_group_name_H-M_alt        'I 4 2 2'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2017-04-12 deposited with the CCDC.
2017-07-05 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   24.810(2)
_cell_length_b                   24.810(2)
_cell_length_c                   17.8094(15)
_cell_measurement_reflns_used    6331
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      19.99
_cell_measurement_theta_min      2.16
_cell_volume                     10962.3(16)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'Omega and phi scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0822
_diffrn_reflns_av_unetI/netI     0.0500
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -33
_diffrn_reflns_limit_k_max       33
_diffrn_reflns_limit_k_min       -33
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            58599
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.318
_diffrn_reflns_theta_min         1.161
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    0.481
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.6472
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            'light blue'
_exptl_crystal_density_diffrn    1.203
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             4152
_exptl_crystal_preparation       ', Ferroelectric and Dielectric'
_exptl_crystal_recrystallization_method
'Re-crystallisation from solvent: Methanol and water'
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.455
_refine_diff_density_min         -0.260
_refine_diff_density_rms         0.063
_refine_ls_abs_structure_details
;
 Flack x determined using 1224 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.036(12)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.066
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     218
_refine_ls_number_reflns         6848
_refine_ls_number_restraints     62
_refine_ls_restrained_S_all      1.080
_refine_ls_R_factor_all          0.1308
_refine_ls_R_factor_gt           0.0668
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1420P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1981
_refine_ls_wR_factor_ref         0.2478
_reflns_Friedel_coverage         0.804
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.999
_reflns_number_gt                3638
_reflns_number_total             6848
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7tc01758h2.cif
_cod_data_source_block           compound_1_sq
_cod_original_cell_volume        10963(2)
_cod_database_code               7236800
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              97782
_shelx_hkl_checksum              83864
_shelx_fab_checksum              36323